Redetermination of β-Al~2~TiO~5~ obtained by melt casting
Stefan T. Norberg; Nobuo Ishizawa; Stefan Hoffmann; Masahiro Yoshimura; Acta Crystallographica Section E 61 (2005) i160–i162; doi:10.1107/S1600536805021331

data_2206495
_publ_section_title
;
 Redetermination of \b-Al~2~TiO~5~ obtained by melt casting
;
_journal_coeditor_code           MG6041
_journal_issue                   8
_journal_name_full               'Acta Crystallographica Section E'
_journal_page_first              i160
_journal_page_last               i162
_journal_paper_doi               10.1107/S1600536805021331
_journal_volume                  61
_journal_year                    2005
_chemical_formula_iupac          'Al2 Ti O5'
_chemical_formula_moiety         'Al2 O5 Ti'
_chemical_formula_structural     'Al2 O5 Ti'
_chemical_formula_sum            'Al2 O5 Ti'
_chemical_formula_weight         181.84
_space_group_IT_number           63
_symmetry_cell_setting           orthorhombic
_symmetry_space_group_name_Hall  '-C 2c 2'
_symmetry_space_group_name_H-M   'C m c m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   3.605(2)
_cell_length_b                   9.445(4)
_cell_length_c                   9.653(4)
_cell_measurement_reflns_used    8632
_cell_measurement_temperature    297.0(10)
_cell_measurement_theta_max      30.53
_cell_measurement_theta_min      3.02
_cell_volume                     328.7(3)
_computing_cell_refinement       RAPID-AUTO
_computing_data_collection       'RAPID-AUTO (Rigaku, 2003)'
_computing_data_reduction
;
RAPID-AUTO (Rigaku 2003), and DIFDAT, SORTRF and ADDREF in Xtal3.7 (Hall
<i>et al.</i>, 2000)
;
_computing_molecular_graphics
'DIAMOND (Brandenburg, 2001), and FOURR, SLANT and CONTRS in Xtal3.7'
_computing_publication_material  'BONDLA, ATABLE and CIFIO in Xtal3.7'
_computing_structure_refinement  'CRYLSQ in Xtal3.7'
_computing_structure_solution
'atomic positions from Morosin & Lynch (1972)'
_diffrn_ambient_temperature      297.0(10)
_diffrn_measured_fraction_theta_full 1.00
_diffrn_measured_fraction_theta_max 1.00
_diffrn_measurement_device_type  'Rigaku R-AXIS RAPID'
_diffrn_measurement_method       \w
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'normal-focus sealed tube'
_diffrn_radiation_type           'Mo K\a'
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.025
_diffrn_reflns_av_sigmaI/netI    0.02
_diffrn_reflns_limit_h_max       5
_diffrn_reflns_limit_h_min       -5
_diffrn_reflns_limit_k_max       13
_diffrn_reflns_limit_k_min       -13
_diffrn_reflns_limit_l_max       13
_diffrn_reflns_limit_l_min       -13
_diffrn_reflns_number            1774
_diffrn_reflns_theta_full        30.47
_diffrn_reflns_theta_max         30.47
_diffrn_reflns_theta_min         4.22
_diffrn_standards_decay_%        0
_diffrn_standards_interval_count 0
_diffrn_standards_interval_time  0
_diffrn_standards_number         0
_exptl_absorpt_coefficient_mu    3.019
_exptl_absorpt_correction_T_max  0.880
_exptl_absorpt_correction_T_min  0.827
_exptl_absorpt_correction_type   gaussian
_exptl_absorpt_process_details   '(RAPID-AUTO; Rigaku, 2003)'
_exptl_crystal_colour            blue
_exptl_crystal_density_diffrn    3.675
_exptl_crystal_description       block
_exptl_crystal_F_000             352
_exptl_crystal_size_max          0.088
_exptl_crystal_size_mid          0.073
_exptl_crystal_size_min          0.055
_refine_diff_density_max         0.91
_refine_diff_density_min         -0.73
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_all   1.093
_refine_ls_goodness_of_fit_ref   1.112
_refine_ls_matrix_type           full
_refine_ls_number_constraints    21
_refine_ls_number_parameters     28
_refine_ls_number_reflns         288
_refine_ls_number_restraints     0
_refine_ls_R_factor_all          0.030
_refine_ls_R_factor_gt           0.028
_refine_ls_shift/su_max          0.00019
_refine_ls_shift/su_mean         0.000015
_refine_ls_structure_factor_coef F
_refine_ls_weighting_details     'w = 1/[\s^2^(F) + 0.015(F)]'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_all         0.029
_refine_ls_wR_factor_gt          0.028
_refine_ls_wR_factor_ref         0.028
_reflns_number_gt                288
_reflns_number_total             304
_reflns_threshold_expression     F>2\s(F)
_cod_data_source_file            mg6041.cif
_cod_data_source_block           I
_cod_database_code               2206495